Bioengineering of CuO porous (nano)particles: role of surface amination in biological, antibacterial, and photocatalytic activity

Nanotechnology is one of the most impressive sciences in the twenty-first century. Not surprisingly, nanoparticles/nanomaterials have been widely deployed given their multifunctional attributes and ease of preparation via environmentally friendly, cost-effective, and simple methods. Although there are assorted optimized preparative methods for synthesizing the nanoparticles, the main challenge is to find a comprehensive method that has multifaceted properties. The goal of this study has been to synthesize aminated (nano)particles via the Rosmarinus officinalis leaf extract-mediated copper oxide; this modification leads to the preparation of (nano)particles with promising biological and photocatalytic applications. The synthesized NPs have been fully characterized, and biological activity was evaluated in antibacterial assessment against Bacillus cereus as a model Gram-positive and Pseudomonas aeruginosa as a model Gram-negative bacterium. The bio-synthesized copper oxide (nano)particles were screened by MTT assay by applying the HEK-293 cell line. The aminated (nano)particles have shown lower cytotoxicity (~ 21%), higher (~ 50%) antibacterial activity, and a considerable increase in zeta potential value (~ + 13.4 mV). The prepared (nano)particles also revealed considerable photocatalytic activity compared to other studies wherein the dye degradation process attained 97.4% promising efficiency in only 80 min and just 7% degradation after 80 min under dark conditions. The biosynthesized copper oxide (CuO) (nano)particle’s biomedical investigation underscores an eco-friendly synthesis of (nano)particles, their noticeable stability in the green reaction media, and impressive biological activity.

www.nature.com/scientificreports/ In nanomedicine, there are numerous advantages in employing plants as natural and renewable resources for the green synthesis of metal nanoparticles. Such an ideal approach for the nanofabrication of CuO brings value and may pave the way for biomedical applications. In such biological processes, the toxicity of utilized reagents for the nanoparticle's synthesis is relatively low, and natural elements are deployed for reducing, capping, and stabilizing the metal's nanoparticles. Natural materials such as plants and agricultural residues and waste encompassing compounds like quinines, alkaloids, terpenoids, flavonoids, fatty acids, enzymes, amino acids, phenols, and tannins have distinctive roles in the synthesis of nanoparticles. The biological method is environmentally friendly and leads to highly efficient and cost-effective synthesis and has been extensively used in assorted applications such as drug delivery, gene therapy, nanobiotechnology, medicine, biomedical engineering, and pharmacology [14][15][16][17][18][19] .
Although chemical and physical synthesis methods have been vastly utilized for the preparation of nanoparticles, being non-eco-friendly, and involving hazardous material usage diminishes their acceptance. In this regard, the bioengineered synthesis methods could replace these methods as they exploit plant phytochemicals or microbial enzymes. Among biologically synthesized nanoparticles (graphene oxide, iron oxide, zinc oxide, platin, selenium, gold, silver), CuO nanoparticles have garnered attention because they comprise a co-factor of the plethora of human neuropeptide enzymes, and are involved in immune cell function, anti-oxidant defense, and cell signaling regulation 20 .
The bioengineering synthesis process can be divided into three main categories (i) using plant and plant extract (phyto route), (ii) utilizing microorganisms like actinomycetes, bacteria, yeasts, and fungi (microbial pathway), and (iii) usage of templates such as diatoms, viruses, and membrane (bio-template route). The pathway utilizing the abundant plant extractives is preferred to other means because of greener attributes and being well dispersed, endowed with a faster pace of synthesis and relatively lower cytotoxicity; the plant extracts can provide electrons that help reduce the copper salt and also serve as stabilizing agents 21 . Some of the major contributions to the assembly of CuO nanoparticles via a bioengineered pathway are summarized in Table 1.
In the past few decades, various bacterium and viral disease have been treated with metals/metal oxide nanoparticles wherein CuO nanoparticles have displayed considerable antibacterial activities; CuO nanoparticles being highly toxic to the plethora of plant or human bacterial pathogens 49 in view of their high chemical and biological reactivity, biocompatibility, high surface area, and small size 50 . When CuO nanoparticles come in contact with bacterium cells with help of amines and carboxylic groups on cell membrane, an effortless entry inside the cell occurs with the development of several malfunction cytotoxicity 51 . CuO nanoparticles generate ROS (reactive oxygen species) that can disrupt the membrane and interfere with cell division, metabolism, and DNA replication besides the degradation of ribosomes and mitochondria promoted by CuO nanoparticlesmediated cytotoxicity. The large redox potential of Cu leads to the generation of the Cu ions and these highly toxic ions accumulate the hydroxyl and superoxide radicals (oxidative stress) 52 . Chtita et al. 29 fabricated a CuO nanoparticle utilizing Gloriosa superba leaf extract that revealed good inhibitory against Klebsiella aerogenes (gram-negative bacteria) and Staphylococcus aureus (gram-positive bacteria) 53 . Sida acuta leaf extracts has been used by Sathiyavimal and colleagues for the fabrication of CuO nanoparticles as they applied these biosynthesized compounds in the cotton fabrics against gram-negative and gram-positive bacterium with promising results 22 . Green synthesized CuO nanoparticles from the precursor, Cu (CH 3 COO) 2 by Nwaya et al. demonstrated promising growth inhibitory activity against various species of pathogenic bacteria such as Pseudomonas aeruginosa and Bacillus licheniformis 29 .
One of the new era's catastrophic problems is water pollution which has been a major concern for society; it has garnered much attention for the purification of wastewater. Unique features of nanomaterials make them perfect candidates for the degradation of water pollutants like dyes as these photocatalysts are efficient, inexpensive, and offer sustainable approach in wastewater treatment. Photocatalysis is based on having a band gap between the valence band (VB) and the conduction band (CB). When the excited electrons travel from VB to CB, electron-hole (e − /H + ) pairs are generated and transferred to the surface of the catalyst and react with other materials such as O 2 and H 2 O; In VB and CB, e − and H + are able to generate hydroxyl radical (·OH) and O 2 − , respectively which are responsible for the degradation of pollutants [54][55][56] . For example, Iqbal and coworkers synthesized CuO nanoparticles using an aqueous extract of Rhazya stricta and investigated it in the degradation of methylene blue (MB) wherein CuO NPs caused 83% degradation of MB after 140 min of reaction 57 . Some of the unique studies are listed in Table 3.
In this study, we have focused on the synthesis and characterization of CuO (nano)particles utilizing the Rosmarinus officinalis leaf extract. Besides, their photocatalytic and biological activity including the cytotoxicity and antibacterial assessment against Bacillus as a Gram-positive and Pseudomonas as a Gram-negative bacterium, was evaluated.

Materials and methods
Reagents, chemicals, and plant source. All  The plant extract preparation. The Rosmarinus officinalis was washed with distilled water and then kept at room temperature to dry 20 . The powdery form of the dried plant was prepared by grinding, and the fine pulverized powder (10 g) was dispersed in deionized water (100 mL) and placed for 15 min on a heater stirrer at the boiling point of the solvent and then, set at room temperature for cooling. The Whatman filter paper (grade one) used for filtration of the final solution and the prepared extract have been stored for further experiments at a 4 °C 46,60,61 .

Synthesis of CuO (nano)particles. For the synthesis of copper oxide (nano)particles from the leaves of
Rosmarinus officinalis, 40 mL of extract of Rosmarinus officinalis was transferred to the cupric sulfate solution (160 mL, 1 mM), and after a while, the color changed from mild blue to dark one; mixture being agitated at 25 °C for 24 h. The leaf extract played two crucial roles in this study, as a stabilizing agent and a reducing agent wherein the capping of (nano)particles with ketone and aldehyde groups can control the growth, aggregation, and also reduction process; plant extract has a huge impact on the shape, size, and morphology of the ensued (nano)particles. Based on reported data, higher the concentration of the plant extract, the smaller is the size of ensued (nano)particle, which is a consequence of the presence of additional phytoconstituents. The product was characterized by different techniques such as FT-IR, UV-Vis, and PXRD ( Fig. 1).
For separation of unreacted materials and byproducts from the reaction mixture and the CuO (nano)particles, the solution was centrifuged for 25 min at 10,000 rpm and then washed with deionized water and ethanol (three times). The copper oxide-dried powder was obtained by freeze-drying. The technique of ultra-centrifugation was utilized to separate (nano)particles based on their size 62-64 . Chlorination of copper oxide (nano)particles. Chlorine is one of the most promising ligands in coordination chemistry, which facilitates further functionalization. Accordingly, 15 mL of thionyl chloride was added to the filtered-off product (CuO (nano)particles); additionally, to increase the rate of reaction, 2 mL of DMF was added (18 h, yellow solid, argon atmosphere). Then to obtain a dried powder, the solution was kept in the oven for 24 h. Antibacterial activity. Antibacterial activities of the compounds against Bacillus cereus and Pseudomonas aeruginosa were assessed by the renowned disk diffusion method utilizing Müller Hinton agar and Sabouraud Dextrose Agar (SDA). The inhibition zone on the incubation completion has been recorded, and the average diameter for every compound was recorded at 400 μg mL −1 , and the dimethyl sulfoxide (DMSO)-based Stock solutions of compounds were prepared. Standard antibiotics like penicillin, ampicillin, and gentamicin with similar concentrations have been utilized to compare with compound inhibition zone. To minimize the error, each test was carried out several times (at least three times). As the effect of the DMSO at the biological screening should be clarified, blank studies have been accomplished, and no activity was observed in pure DMSO against any bacterial strains 65,66 .
Photocatalytic activity. The photocatalytic activity of CuO-NH 2 (nano)particles was evaluated in an aqueous solution by calculation of methylene blue degradation. For this purpose, the utilized light source was a 250-W mercury lamp to prepare visible light with a wavelength of more than 420 nm. An optical glass (400-800 nm cutoff filter) was used to determine photocatalytic activity. The photocatalytic tests were carried out with a 100 mL photoreactor at STP 67 . Every analysis was performed using 0.3 g/L of dispersed CuO-NH 2 as the photocatalyst in the 10 mg/L methylene blue aqueous solution. The mixture was stirred and exposed under irradiation simultaneously. To calculate the methylene blue concentration, at the regular steps (exact time interval), 4 mL of solution was separated and screened at 600 and 670 nm (absorbance wavelength) 68,69 . www.nature.com/scientificreports/ MTT assay. The cytotoxicity of synthesized (nano)materials has been investigated by applying the HEK-293 cell line. In brief, 100 µL of F12/DMEM was supplemented with ten percent FBS and incubated in a 96-well plate seeded with 10 5 cell density per well. The fresh media of several diluted prepared (nano)particles replaced the culture media then newly prepared cells were incubated for 5 h. As mentioned above, the media is replaced with fresh media (for 24 h) at the next stage. After four h incubation at STP, the prepared media aspirated and, in this stage, generated MTT formazan has been dissolved in Dimethyl sulfoxide. Every well's absorbance has been recorded at 570 nm using a microplate reader [70][71][72][73] .
Leaves collection permission. The Rosmarinus officinalis have been obtained from Kurdistan province in Iran, and all of the National Laws and/or protocols have adhered appropriately. Amir Mohamad Ghadiri collected the plant samples, and obtained local permissions.

Results and discussion
Synthesis and characterization. Considering the FT-IR spectrum ( Fig. 2A), the broad bands are revealed at ~ 3380 cm −1 representing the hydroxyl group stretching frequency (hydroxyl groups on the surface of the CuO (nano)particles). The Cu-O bonds stretching vibration indicator has been revealed 74,75 on the 686 cm −1 .
The peak at 2925 cm −1 proved the presence of carboxylic acid O-H stretching, while another one at 1566 cm −1 is for aliphatic nitro compounds. In CuO-Cl spectra, a band at about 870 cm −1 belongs to C-Cl. Also, the peak at 2421 cm −1 (thiol S-H stretch) is not observed in CuO-NH 2 spectra, which showed the replacement of amide and thiol on the surface of copper oxide (nano)particles. Additionally, in CuO-NH 2 spectra, the bands observed at ~ 2900 cm −1 is accredited to N-H bonding contributed by 1,4-phenylenediamine on CuO (nano)particles. Their stability after photocatalysis process is affirmed by the subsequent FT-IR analysis of CuO-NH 2 (nano)particles as depicted in the Fig. 2A which is reliable evidence of (nano)particles stability ( Table 2)   www.nature.com/scientificreports/ PL spectroscopy has been widely applied to evaluate the rate of recombination of photogenerated electron-hole pairs on irradiated semiconductor nanoparticles 85 . One of the significant points is that the PL intensity has a direct relation with the electron-hole pair recombination rate. In general, it is well known that as the PL intensity becomes weaker, the recombination rate in semiconductors decreases; as a result, the lifetime of photogenerated charge carriers increases significantly, which causes the better photocatalytic activity of the desired photocatalyst. Figure 2D exhibits the PL spectra of CuO, CuO-Cl, and CuO-NH 2 nanoparticles at the maximum excitation wavelengths of these nanoparticles (Fig. 2C). As can be clearly seen in the figure, the PL intensity spectrum of CuO-NH 2 NPs is relatively lower than that of CuO-Cl and CuO nanoparticles. Also, the PL intensity spectrum of CuO-Cl nanoparticles is relatively lower than that of pure CuO nanoparticles. These results clearly illustrate that the electron-hole pair recombination can be significantly reduced by modifying the surface of copper oxide nanoparticles with chlorine and amine. The inhibition of electron-hole pair recombination by the surface amine group leads to a more efficient separation of photo-generated charge carriers, which eventually increases the photocatalytic activity of semiconducting NPs. Compared with pure copper oxide NPs and chlorinated copper oxide NPs, aminated copper oxide NPs exhibited a remarkable quenching in the PL intensity emission signal, which indicates that the amination of copper oxide NPs can lead to better separation efficiency of photo-generated charge carriers and consequently enhance the efficiency of photocatalytic activity of semiconducting nanoparticles.
The FESEM analysis has been utilized to evaluate the synthesized (nano)particle's morphology. The FESEM images of the synthesized CuO (nano)particles mediated by Rosmarinus officinalis leaf are depicted in Fig. 3A1-A3, the aminated CuO (nano)particles being shown in Fig. 3B1-B3. The homogenous size range and monodispersed distribution are the features of these biosynthesized copper oxide (nano)particles. Stabilizing agents as well as reducing agents can change the morphology and the shape of (nano)particles both of them being performed by the plant extract in this case. The ensued data are in agreement with recent descriptions of copper oxide nanoparticles [78][79][80][86][87][88] . The Fig. 3C1-C3 is related to the CuO-NH 2 (nano)particles after photocatalysis activity which illustrates that the surface morphology of prepared (nano)particles did not change considerably relative to the pristine CuO-NH 2 surface morphology, which presents compelling evidence of (nano)particle's stability. The DLS results demonstrate that the amination process can lead to increase of the particle size, and it could be due to increasing the hydrogen bands (Figs. S5-S7). Table 2. The survey on the recent advancements on the biomedical potentials of the CuO nanoparticles. "− " and "+ " represent the absence and presence of the activity.   www.nature.com/scientificreports/ The elemental analysis (EDS) and elemental mapping are presented in Fig. 4A-X which revealed that all elements are well distributed on the (nano)particles' surface, their percentage changing in considerable concordance with the synthesis steps. The zeta potential of prepared CuO and CuO-NH 2 (nano)particles were − 8.4 and + 5 mV that; this considerable difference, was in good accordance with EDS results (elements' percentage change) (Figs. S3 and S4).
Antibacterial activity. There are some probable mechanisms for antibacterial activity of metal nanoparticles such as disruption of cell membrane, DNA and protein damage, cell substances oxidation, attachment to ribosome, generation of ROS (reactive oxygen species), prevention of biofilm production, proton efflux damage, penetrating and then connection of metal ion to the cell's sulfur and phosphorus which leads to apoptosis and connection of metal ion to the thiol group of the cell-surface protein. However, the precise mechanism is unknown, the further biological studies are necessary to broaden the available data. The prepared compounds have been tested for antibacterial activity against Pseudomonas aeruginosa gram negative species and Bacillus cereus as Gram positive. The amination of the CuO (nano)particles leads to ~ 50% increasing in antibacterial activity for example, the aminated CuO (nano)particles inhibition zone on Pseudomonas aeruginosa is about 29 mm while, the inhibition zone of CuO (nano)particles is 20 mm. The solvent and the extract of plant do not show momentous activity, it is proven that these compounds show antibacterial activity in comparison with that detected for standard antibiotic gentamicin, penicillin, and ampicillin. The results are compared with other researches and the collected data is quite considerable (Fig. 5). The ROS generated by CuO NPs can interact with bacteria's cell membrane for penetrating to the cell and this connection can make some malfunction that inhibit the bacterial growth and leads to cell death. The smaller the size of (nano)particles, easier is the entry without any interference. The abundant functional groups such as amine and carboxyl on the surface of the cell Photocatalytic activity. The photocatalysis has been proposed for abatement the environmental pollutants and nowadays it is playing pivotal role as it is relatively non-toxic, efficient, and inexpensive. Three step essentially comprise the reactions which occur on the surface of photocatalyst: (i) absorption of the light, (ii) disconnection and transfer of photogenerated electrons, (iii) and redox reaction. The main argument about the dye degradation mechanism is that oxygen and superoxide radicals are produced from the reaction of photogenerated electrons and hydroxyl radicals which then degrade the methylene blue (MB) dye. The CuO-NH 2 (nano)particles photocatalytic activity have been screened by the degradation of methylene blue. The prepared (nano)particles were transferred to the dye-containing solution, and the mixture was irradiated by the lamp, as mentioned earlier (visible light) 67 . The UV-Vis spectra (Fig. 6A) revealed that the dye degradation (decrease in maximum absorbance) of MB in the presence of synthesized (nano)particles (CuO-NH 2 ) occurred after 80 min with 97.4% efficiency which is significant result among all CuO-based nanoparticles. Based on the outcome of studies, the time and the yield of degradation process by aminated CuO were found to be the best (Table 3) 98 .
In this work, before performing the photocatalysis process in presence of light, we screened CuO-NH 2 photo degradation efficiency under dark condition (Fig. 6B). Under dark conditions, it caused only ~ 7% degradation after 80 min. On the other hand, in the presence of light, more than 97% degradation is recorded thus clarifying that the light is responsible for the degradation of methylene blue 99 .
Photodegradation process for methylene blue (MB). The plausible photocatalytic mechanism for the photodegradation of MB dye by synthesized CuO-NH 2 NPs is presented in Fig. 7. Irradiation of visible light to the CuO-NH 2 NPs' catalytic surface causes the movement of photoexcited electrons from the VB to the CB and produces electron-hole pairs, as displayed in Eq. (1):  In the conduction band, due to the reduction process of the oxygen molecules, superoxide free radicals are produced, and finally, these produced radicals are converted into hydroxyl free radicals in several consecutive steps, as displayed in Eq. (3) 103 : Eventually, the photodegradation of desired dye occurs via the produced active ·OH free radicals, as displayed in Eq. (4): The photodegradation of MB dye entails several steps up to generate the H 2 O and CO 2 molecules eventually. The photodegradation of organic pollutants is accomplished by powerful oxidants such as ·OH radicals, which are shown in Fig. 7 104 . Cytotoxicity. It is obvious that the prepared (nano)material's cellular safety must be considered in advance of any potential biomedical appliance. The cytotoxicity of copper oxide nanoparticles has been reported in some papers, but the lack of utilization of a green method could increase the cytotoxicity. Based on other studies, the cytotoxicity of Rosmarinus officinalis leaf 's extract was quite low and the cell viability was relatively high. On the contrary, the cytotoxicity of CuO (nano)particles is higher and their cell viability is lower. Based on the zeta potential results, the surface amination has led to considerable increases in surface potential (Figs. S3 and S4) 105 . It is evident that by making the surface potential more positive, the cytotoxicity of compounds will drastically decrease and The MTT assay results of aminated product clearly has affirmed this claim. The more positive surface, makes the prepared compound a good candidate for drug and gene delivery. So, the proposed method (surface amination) can be utilizable in various nanosystem for biomedical purposes. The cell viability of CuO- www.nature.com/scientificreports/ NH 2 is conspicuously higher (~ 21%) while the cytotoxicity is considerably lower. The prepared (nano)material's stability and safety has been confirmed by convergent trend results of 24-and 48-h treatment (Fig. 8A,D). Also, the heat map graphs are depicting the interrelationship among (nano)materials various concentration and relative cell viability (Fig. 8B,E). The dose-dependent response of prepared (nano)materials is proved by MTT assay with utilized the (nano)materials at varying concentrations namely 0.1, 0.5, 1, 5, 10, 50 µg/mL; Fig. 8C

Conclusion
The present study focuses on the biosynthesis of aminated copper oxide (nano)particles from Rosmarinus officinalis leaf extract for the first time wherein an inclusive study about the potential biological and photocatalytic activity was undertaken. The prepared (nano)particles have been fully characterized and revealed a promising photocatalytic activity on degradation of methylene blue dye (~ 97% degradation under light in 80 min and just ~ 7% in dark condition and 80 min). These biosynthesized (nano)particles displayed potential antibacterial activity as well when screened against Bacillus as a gram-positive and Pseudomonas as a gram-negative bacterium (~ 50% increase in antibacterial activity for CuO-NH 2 compared to CuO (nano)particles). The encouraging results are due to the synthesis technique deployed for the metal oxide nanoparticles and, specifically, the first aminated copper oxide (nano)particles with this promising potential. It is quotable that the amination of CuO led to considerable increase (Δζ = + 13.4 mV) in zeta potential of prepared (nano)particles. Additionally, the MTT assay investigation of the biosynthesized aminated copper oxide (nano)particles revealed that the proposed modification method leads to lower cytotoxicity (~ 21%). Owing to the considerable stability of prepared nanoparticles in greener media and based on remarkable results in vitro studies, the impressive ensued biological activity are additional attractive features of this study.

Data availability
All data generated or analyzed during this study are included in this published article.  www.nature.com/scientificreports/ Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons licence, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons licence, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons licence and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this licence, visit http:// creat iveco mmons. org/ licen ses/ by/4. 0/.